EM 388F – Fracture Mechanics Term Paper p Fracture of Orthotropic Materials under Mixed Mode Loading Julian Hallai Apr 30th 2008 Apr 30 Outline • • • • • • Wood as orthotropic material Wood as orthotropic material Overview of fracture in wood Fracture toughness in mode I and mode II h i d d d Mixed mode fracture criteria Comparison with experimental data Conclusions Wood as Orthotropic Material Wood as Orthotropic Material • Wood Wood is generally considered a cylindrically is generally considered a cylindrically orthotropic material, with the principal axes of orthotropy (R,T,L) given by the radial, tangential and longitudinal directions Elastic Moduli Elastic Moduli Constitutive Relation Constitutive Relation Strength • In In the radial and the radial and tangential directions the strength is 10‐30% of that in longitudinal direction • There is also difference between tensile and compressive strengths compressive strengths. Fracture Orientations Fracture Orientations Across the grain Parallel to the grain the grain Fracture along the Grain Fracture along the Grain • Cracks Cracks in wood generally grow along the in wood generally grow along the grains irrespective of both the original orientation of the crack and the mode mixity orientation of the crack and the mode mixity • Even when cross‐grain notches are loaded in longitudinal tension cracking usually occurs longitudinal tension, cracking usually occurs along the grain (perpendicularly to the notch) • Orientations RL and TL are usually the primary Oi i RL d TL ll h i focus. Tension at Arbitrary Angles Relative to the Grain l h • Due to anisotropy, it is py, essentially impossible to get a pure mode I. Mixed mode condition arises! mode condition • Cracks will propagate along the weak axes of the material but h lb frequently jump between g grain lines when doing so g maximizes the energy release. Fracture Toughness Fracture Toughness Mixed Mode Fracture Mixed Mode Fracture • Crack Crack growth depends on not only K growth depends on not only KIC and KIIC but IC and K IIC but also on the interaction between the two • Theories for predicting mixed mode fracture in p g anisotropic homogeneous materials usually predict that a crack subjected to mixed mode loading will grow out of its original plane. They cannot be directly applied to wood Mixed mode fracture Mixed mode fracture • In In isotropic materials, isotropic materials, the crack will typically turn so that its plane is perpendicular to the load axis, becoming mode I. d I • In case of wood, it will continue to propagate continue to propagate under mixed mode. Mixed mode fracture criteria Mixed mode fracture criteria • Empirical criterion Empirical criterion – based on experiments with balsa wood and fiber‐ glass‐reinforced glass reinforced plastic plates plastic plates Mixed mode fracture criteria Mixed mode fracture criteria • Empirical criterion Empirical criterion – Eastern Red Spruce 2 < b < 3.5 Mixed mode fracture criteria Mixed mode fracture criteria • Critical Energy Release Rate Critical Energy Release Rate – fracture takes place when the strain energy release rate during crack propagation equals the release rate during crack propagation equals the energy rate needed to tear the material apart. Mixed Mode Fracture Criteria Mixed Mode Fracture Criteria • Critical Strain Energy Density Critical Strain Energy Density – Crack growth occurs when the strain energy density at some distance from the crack tip density at some distance from the crack tip reaches a critical value. Mixed Mode Fracture Criteria Mixed Mode Fracture Criteria • Critical In Critical In‐Plane Plane Maximum Principal Stress Maximum Principal Stress – Fracture takes place when the maximum principal stress at some distance in front of the crack tip stress at some distance in front of the crack tip reaches a critical value. Mixed Mode Fracture Criteria Mixed Mode Fracture Criteria • Non Non‐local local Stress Fracture Criterion (2008) Stress Fracture Criterion (2008) – Fracture takes place when the mean value of the function of decohesive normal and shear stress function of decohesive normal and shear stress over a segment d, the length of the damage zone, reaches its critical value Crack parallel to the grain Crack arbitrarily oriented Discussion Scots Pine Scots Pine Eastern Red Spruce Eastern Red Spruce Experiment Experiment Energy Release Rate Energy Release Rate Strain Energy Density Strain Energy Density Max Principal Stress Max Principal Stress Discussion Norway Spruce y p Discussion Pine Wood – crack arbitrarily oriented y Conclusions • Empirical criteria require a large number of p ca c te a equ e a a ge u be o material constants determined for each crack configuration. • The energy based criteria don’t predict well the mixed mode fracture in wood. • Cracks oriented along the grain – Critical In‐Plane Maximum Principal Stress criterion – Non‐Local Stress Fracture Criterion N L l St F t C it i • Cracks oriented arbitrarily • Non‐Local Stress Fracture Criterion Non Local Stress Fracture Criterion References • Ashby, M.F.; Easterling, K.E.; Harrysoon, R.; Malti, S.K. (1985) The fracture and toughness of woods. Proceedings of the Royal Society of London. Series A, Mathematical and Physical Sciences; 398: 261‐280. • Gillis, P. (1972) Orthotropic elastic constants of wood. Wood Science and Technology; 6: 138‐156. • Jernkvist k i LO. O (2001) Fracture off wood d under d mixed i d mode d loading l di I: Derivation i i off fracture f criteria. i i Engineering Fracture Mechanics; 68: 549‐563. • Romanowicz, M.; Seweryn, A. (2008) Verification of a non‐local stress criterion for mixed mode fracture in wood. Engineering Fracture Mechanics, 75: 3141‐3160. • Smith, I.; Landis, E.; Gong, M. (2003) Fracture and fatigue in wood. West Sussex: John Wiley & Sons. • Midess, S.; Bentur, A. (1986) Crack propagation in notched wood specimens with different grain orientations. Wood Science and Technology, 20: 145‐155. • Dimwoodie, J.M. (2000) Timber: Its nature and behavior. 2nd edition. London: E & FN Spon. • Wu, E.M. (1967) Application of fracture mechanics to anisotropic plates. Journal of Applied Mechanics, 34 (4): 967‐74 • Mall, S.; Murphy, J.F.; Shottafer, J.E. (1983) Criterion for mixed mode fracture in wood. Journal of Engineering g g Mechanics,, 109 ((3): ) 680‐690. • Sih, G.C. (1974) Strain‐energy‐density factor applied to mixed mode crack problems. International Journal of Fracture, 10 (3): 305‐321. • Jernkvist LO. (2001) Fracture of wood under mixed mode loading II. Experimental investigation of Picea abies. Engineering Fracture Mechanics; 68: 565 565‐576. 576. • Hutchinson, J.W.; Suo, Z. (1992) Mixed mode cracking in layered materials. Advances in Applied Mechanics, 29: 63‐191.